Head Office: Università degli Studi di Padova
Department of Chemical Sciences
Ph.D. COURSE IN:Science and Engineering of Materials and Nanostructures
Defective and Hybrid 2D-Materials
Coordinator: Ch.mo Prof. Giovanni Mattei Supervisor: Ch.mo Prof. Gaetano Granozzi
1.2 Motivations of Ph.D. project………5
1.2.1 Green Energy: Fuel Cells and Electrochemical Water Splitting ……….……….6
1.2.2 Green Chemistry: Catalyst Heterogenization………..8
1.3 Evolution of 2D Materials and State of the Art………11
1.3.1 First Generation of Graphene: Aiming the Perfection………11
1.3.2 Second Generation of Graphene: Chemically Modified and 3D-Structured Graphene………...11
1.3.3 Third Generation of Graphene: Graphene Related Materials………..14
1.4 Ph.D. Thesis structure………19
Chapter 2: Promotion of the hydrogen evolution kinetics by Ni-doping of 3D-structured MoS2 in acid and alkaline media 2.1 Introduction………..35
2.2 Experimental Section………..36
2.3 Results and Discussion………38
2.3.1 Preliminary study on 3D-MoS2 scaffold………38
2.3.2 Synthesis and physico-chemical characterization ………...39
2.3.3 Electrochemical characterization.………...45
Chapter 3: Highly Efficient MoS2/Ag2S/Ag Photoelectrocatalyst Obtained from a Recycled DVD Surface 3.1 Introduction………..57
3.2 Experimental Section………..58
3.3 Results and Discussion………59
Chapter 4: One-pot solvothermal synthesis of MoS2(1-x)Se2x/N-rGO hybrids for photoenhanced Hydrogen Evolution Reaction 4.1 Introduction………..75
4.2 Experimental Section………..76
4.3 Results and Discussion………78
4.3.1 N-rGO Structural Characterization.……….…78
4.3.2 Morphological Analysis on MoS2(1-x)Se2x/N-rGO hybrid.………...80
4.3.3 Structural and chemical characterization.….………...82
4.3.4 Electrochemical and Photoelectrochemical characterization.….………...85
Chapter 5: Ferrocene covalently functionalized Graphene Acid and Graphene Oxide as arene C-H insertion catalysts
5.2 Experimental Section………..108
5.3 Results and Discussion………111
5.3.1 Functionalization and characterization of the graphenic materials……….…111
5.3.2 Catalytic Experiments……….………...120
5.3.3 NMR data for isolated organic compounds.………..126
Chapter 6: Homo- and cross-coupling palladium nanoparticles – graphene acid system as stable and recyclable bifunctional green catalyst 6.1 Introduction…………..………135
6.2 Experimental Section………..136
6.3 Results and Discussion………138
6.3.1 Pd nanosystems growth on Graphene Acid………..……….…138
6.3.2 Catalytic Experiments……….………...147
6.3.3 NMR data for isolated organic compounds.………..154
Chapter 7: Conclusions 7.1 Conclusions.…………..………161
List of acronyms and abbreviations………..163
List of publications..………..………..165
Energy and Green Chemistry and it was directed at the application of 2D Materials in particular. This thesis is
divided into five main chapters where we presented five exemplary systems in which we focused our attention on different aspects of materials design. Each chapter comprises an introduction and a conclusion section, in which we tried to go into the details of each targeted application and of the specific design strategy employed. However, at the beginning and at the end of the thesis, the reader can find an Introduction and a Conclusion section where we tried to collocate the goals and challenges of this work within a broader context of materials science and catalysis/electrocatalysis.
In our studies in the Green Energy area, we focused on the use of MoS2-based materials in water splitting cathodic half-reaction in order to obtain the best possible performance in hydrogen generation in different conditions. To do that, different strategies were developed to drive the original material to adapt to specific application. In detail, in Chapter Two we investigated the design of three-dimensional MoS2 structures doped with different amount of Ni in order to activate MoS2 for the Hydrogen Evolution Reaction (HER) performed in alkaline environment, which typically hinder this reaction. We carried out an extensive structural characterization in order to establish the role of each type of active sites formed on the material in the HER activity and kinetics. In Chapter Three, we developed an electrodeposition method for preparing amorphous MoS2/Ag2S hybrid using recycled DVD as the support; this revealed as a viable opportunity to turn an abundant waste into an added-value material. After a suitable investigation to understand what kind of material was formed upon electrodeposition, MoS2/Ag2S/DVD was tested for HER in acidic medium. In Chapter Four another kind of hybrid was prepared by designing a one-pot solvothermal synthesis of MoS 2(1-x)Se2x nanosheets grown on N-doped reduced Graphene Oxide (N-rGO). The goal was the control of the optoelectronic properties of the final material, since the combination of MoS2(1-x)Se2x and N-rGO allows to form p-n nanojunctions, which induce an enhancement of HER activity upon illumination with visible light. Then we used different techniques to prove what was the best Se:S ratio to optimize both the absolute performances in HER and the enhancement upon light irradiation.
Regarding Green Chemistry area, we used Graphene Acid (GA) as starting material and we exploited its uniform surface functionalization to prepare materials for heterogeneous catalysis for different reactions, comparing them with the benchmark Graphene Oxide (GO), modified with the same protocol. In Chapter Five, we synthesized a heterogeneous catalyst by covalently grafting Ferrocene (Fc) moieties to –COOH surface groups of GA and GO. The resulting Fc-modified graphene derivatives have been tested as heterogeneous catalysts for the C-H insertion of aryl diazonium salts into several arene substrates. The tests revealed a strong influence of the support, which we could attribute the intrinsic properties of GA. In Chapter Six, we have grown Pd nanoparticles on GA to prepare a catalyst for Suzuki-Miyaura cross coupling reaction. We have studied the effect of surface functionalization on the nanoparticles formation process and on the derived capability on the controlling the size distribution. The catalysts were tested in Suzuki cross coupling in green conditions and we could highlight the influence of nanoparticles size on activity. Moreover, we studied the same catalysts also for boronic acid homocoupling reaction, that can provide similar final products, but in a more atom economically way.
Nowadays, energy is one of the main challenge of our society. Indeed, the continuous population raising, the colossal economy growth of several countries and the more and more energy demanding lifestyles are severely struggling the actual energetic policy based on fossil fuels. Moreover, also the way we manage the energetic resources is under debate, because, even if the actual energetic resources based on fossil fuels would be enough, the consequences of their use are devastating the world welfare by increasing pollution and global warming. The transition to a more sustainable energetic policy is a dramatically urgent issue that the whole scientific community is addressing in a common multidisciplinary way. In this scenario, materials scientists, chemists and physicists are in the forefront, and main efforts are currently focused both on renewable primary energy sources, sustainable methods for energy conversion and more efficient ways to manage the energy services (see scheme below). The International Energy Agency (IEA) yearly releases the World Energy Outlook (WEO), which can be considered the main reference for the world energetic policy.1
Switching to renewable energy sources (i.e. energy that comes from resources which are naturally replenished on a human timescale) is the unique perspective answer that scientific community has found as effective to find a solution to the mentioned world problems. Especially in the last decade, an extraordinary amount of resources have been spent in order to find viable substitutes to fossil fuels. As already anticipated by Jules Verne in its prophetic fantasy book “The Mysterious Island” (1874, where he says that water will be
the coal of the future), water is the most abundant source for hydrogen, and molecular hydrogen is actually
retained the most promising alternative fuel, since its reaction with oxygen provides clean energy, being
A schematic diagram illustrating the concept
of conversion of primary energy sources
into energy services
Primary Energy Source
Fuel or Electricity
water the unique exhaust product. In this context, a sustainable, clean and cost-effective way to produce hydrogen is required to make the so called hydrogen economy feasible.2,3
The most common method to produce large quantities of hydrogen, i.e. steam reforming of methane or light alcohols, is neither clean nor sustainable. In addition, the final product contains small amounts of CO that constitutes a poison for the Pt-based catalysts used in Fuel Cells (FCs), limiting their lifecycles.4
Electrolyzers, based on the electrocatalytic water splitting (WS), are emerging as the best devices to obtain clean hydrogen through hydrogen evolution reaction (HER).5 However, to be exploitable, WS must be boosted by suitable electrocatalysts. Consequently, preparation and optimization of new electrocatalysts for sustainable electrochemical conversion devices is fundamental to bring innovative solution from laboratory to industrial scale and improve the quantity and the quality of the energy we use.
In this context, Materials Science plays a pivotal role, since it can provide an effective approach to prepare and study completely new materials and all the related properties, up to applications. Graphene is the perfect example of this roadmap: it completely shook up scientific community 15 years ago and now it is progressively going toward commercial productions and applications. As reported in Nature Nanotechnology for the 10th anniversary from the seminal work of Geim and Novoselov,6–8 in 2004-2014 decade, from the first isolation of graphene from graphite by using adhesive tape, graphene has been prepared by many different methods (see Figure 1.1) and graphene sheets are now produced in hundreds of tonnes and tens of thousands of square metres. In 2009, only a few USA-based small start-up companies were making large volumes of small graphene sheets. In the following five years, tens of graphene manufacturing companies have sprung up all over the world, which produce not only micrometric graphene sheets but also large-area, high-quality graphene films on an industrial scale. In particular, the production industry of graphene materials in China has been developing very rapidly, and its total annual production capacity of small graphene sheets and graphene films exceeds 400 tonnes and 110,000 m2, respectively, demonstrating how the drastic approach above mentioned can kick off the business of companies.
Figure 1.1. Comparison of the quality and cost of graphene products manufactured by different methods.
Reproduced from Ref. 4.
Motivations of Ph.D. Project
Considering the unsustainable energetic situation, the development of innovative materials to facilitate the transition to fully sustainable energetics is necessary. Generally speaking, the most popular definition of sustainability is that from the Brundtland Report (Our Common Future, by the World Commission on Environment and Development, 1987, p. 43.) which says:
“Sustainable development is development that meets the needs of the present without compromising the ability of future generations to meet their own needs.”
This very general definition of sustainability can be supported by dividing it in three categories:
► Environmental sustainability is the ability to maintain rates of renewable resource harvest, pollution
creation, and non-renewable resource depletion that can be continued indefinitely;
► Economic sustainability is the ability to support a defined level of economic production indefinitely;
► Social sustainability is the ability of a social system, such as a country, to function at a defined level
of social well-being indefinitely.
This Ph.D. project clearly is aimed at large at developing a Green Economy, whose general definition is: an
economy that aims at reducing environmental risks and ecological scarcities, and that aims for sustainable development without degrading the environment. More specifically the project can be fitted in the sub-fields
1.2.1 Green Energy: Fuel Cells and Electrochemical Water Splitting
The concept of Green Energy is as simple in theory as difficult in practice, and it is made by three key components:
► Production: the way we convert the primary sources for our needs. For example, if we produce electricity via combustion of coal, it may be effective but surely not green because the byproducts of the reaction will pollute seriously the atmosphere, harming people and environment. So a green energy production should be effective without generating dangerous byproducts. Renewable energy sources are the best primary sources since they respect our future because they are naturally replenished on a human timescale, such as sunlight, wind, rain, tides, waves, and geothermal heat.9 ► Utilization: it is related to the efficiency and the energy saving of the devices needed by our life-styles. Being at the moment renewable sources still more expensive than fossil ones (there is a great debate on this point), it is crucial anyway to use the energy we produce in the most effective way. ► Environmental Impact: if the energy production should not impact on the environment, devices that
consume that energy should not do it as well. This component is strongly related to utilization, since typically energy saving induce a lower environmental impact (e.g. a car that burns less fuel will release less COx into the atmosphere). In this context, recycling plays a pivotal role since it provides a value to wastes, allowing to save primary resources. The way to consider properly the balance is considering the whole life-cycle assessment of the products and production methods.
In the last two decades, the scientific community is making great efforts to find out realistic and scalable solutions to effectively substitute fossil fuels and conversion energy systems (e.g. fuel cells, FCs), both for stationary and mobile applications. Molecular hydrogen is nowadays retained the most promising alternative fuel since its reaction with oxygen provides clean energy, being water the unique exhaust product. Indeed, FCs work according to the following half-reactions, that are Oxygen Reduction Reaction (ORR) at the cathode and Hydrogen Oxidation Reaction (HOR) at the anode:
+ 4 + 4 → 2
2 → 4 + 4
Generally, ORR is the main challenging reaction, due to the difficulty of transferring simultaneously 4 electrons from the catalyst to the adsorbed species, causing kinetics hindrance. In the ORR process, Pt-based catalysts are the benchmarks for what concern peak performances, but, having low tolerance to byproducts such as methanol/CO, they undergo to a limited operating life (durability), highlighting the urgency for more durable ORR electrocatalysts.10–12 In addition, platinum group metals (PGMs) are nowadays considered as critical raw materials and their replacement is needed as well.13,14
In this context, a sustainable, clean and cost-effective way to produce hydrogen is required to put the basis for the already mentioned hydrogen economy15. Electrolyzers, based on the electrocatalytic WS, are nowadays commercial devices (still in the phase of optimization) to obtain clean hydrogen through HER at the cathode,5 giving as “byproduct” molecular O
2 at the counter electrode through Oxygen Evolution Reaction (OER). Therefore, the ideal technological loop consists of WS in an electrolyzer through the HER and
OER for fuel generation, followed by power generation through the ORR and HOR in fuel cells, giving green solutions for energy production and utilization (see Figure 1.2) .
Figure 1.2. Scheme of ideal energy loop based on hydrogen generation/storage/utilization.
The overall electrocatalytic reaction of WS is very simple in principle:
: → + ∆ 1.23
Where ΔG is equilibrium for water electrolysis (i.e. the thermodynamical limit), therefore in ideal conditions with ideal electrodes WS could be achieved by applying a small overpotential above 1.23 V. But kinetics can complicate such a simplicity.
The overall reaction can be split in two half-reactions, HER is the cathodic process, whereas OER is the anodic one. Even if overall reaction remain the same, half-reactions are pH-dependent because of the change of species to react in the electrolyte.
In alkaline conditions (pH 14) the corresponding half-reactions are:16
4 + 4 → 2 + 4 ° 0.826
4 → + 2 + 4 ° 0.404
where E°c and Eoa are the equilibrium half-cell potentials at standard conditions of 1 atm and 25 °C.
In neutral solutions (pH 7): 4 + 4 → 2 + 4 ° 0.413 2 → + 4 + 4 ° 0.817 In acidic electrolyte (pH 0): 4 + 4 → 2 ° 0.00 2 → + 4 + 4 ° 1.23
Actually, the main problem of WS is water itself, because of its stability. Indeed, water electrolysis is relatively favourable in acid and alkaline conditions due to the presence of deprotonated water molecules available for OER in alkaline solutions or protonated water molecules for HER in acid solutions. Therefore, in acidic
environment HER would be favoured because the active species would be H3O+ while OER is slowed down and viceversa in basic conditions. This also explains why water electrolysis in neutral condition is kinetically more difficult.
However, since the OER is kinetically more critical than HER, the complete WS has not the same overall efficiency in acid or base. Indeed, OER has to go through a kinetically sluggish 4 electrons process, being unfavourable for removing of four electrons to form O=O bond.17 Therefore, the tendency is to optimize the electrocatalysts for WS in basic conditions. So, to summarize, the more urgent reactions to study are OER and HER in alkaline environment to achieve a feasible large-scale WS. However, HER in acidic electrolyte has to be considered as well, since, in principle, is possible to achieve excellent H2 generation, but substitution of rare and expensive PGMs is mandatory in order to enlarge the production scale.
At the moment, noble metals are the benchmarks for these reactions, in particular Pt is the reference for HER, while Ir- and Ru-based oxides are for the OER. However, as already mentioned, there is a strong issue in maintaining PGMs at the basis of sustainable electrocatalytic processes. This has given rise to a global race for developing innovative electrocatalysts based on non-PGMs materials, which would be also difficult to manage in acidic conditions.
In the present thesis we are focusing on 2D materials for WS. As will be deeper discussed below, these materials, compared to others such as nanowires or nanoparticles, show two important features when considered as electrocatalysts: they are tunable and uniformly expose lattice plane while having unique electronic properties.18 Moreover, 2D materials have significantly high specific surface areas and robust mechanical properties, ideal properties for platforms for practical applications.19 For instance, most layered materials are easily fabricated into freestanding films with uniform thickness.20,21 Compared to powdered catalysts, freestanding electrodes are much more suitable for actual utilization as they can prevent catalyst agglomeration and exfoliation from supports.22 In section 1.3 we will outline the current status of such materials, particularly aiming at their use in electrocatalysis and catalysis.
1.2.2 Green Chemistry: Catalyst Heterogenization
Green Chemistry is a branch of chemistry and chemical engineering that regards the design of chemical
reactions and processes with the goal of lowering the environmental impact of chemistry and applies across the life cycle of a chemical product, including its design, manufacture, use, and ultimate disposal. Clearly, this process goes through the utilization of safer and environmental friendly chemicals and the reduction or the elimination of hazardous byproducts.23
Moreover, the use of renewable material feedstocks and energy sources and the design of energy efficient processes are required. This fact becomes more evident considering that one of the largest energy demands of our society is due to the production of fine chemicals, which accounts for approximately 25% of industrial energy consumption.24
Developed by Paul Anastas and John Warner,25 the following list of 12 principles outlines an early conception of what would make a greener chemical, process, or product:
It is better to prevent waste than to treat or clean up waste after it has been created. 2. Atom Economy
Synthetic methods should be designed to maximize the incorporation of all materials used in the process into the final product.
3. Less Hazardous Chemical Syntheses
Wherever practicable, synthetic methods should be designed to use and generate substances that possess little or no toxicity to human health and the environment.
4. Designing Safer Chemicals
Chemical products should be designed to affect their desired function while minimizing their toxicity. 5. Safer Solvents and Auxiliaries
The use of auxiliary substances (e.g., solvents, separation agents, etc.) should be made unnecessary wherever possible and innocuous when used.
6. Design for Energy Efficiency
Energy requirements of chemical processes should be recognized for their environmental and economic impacts and should be minimized. If possible, synthetic methods should be conducted at ambient temperature and pressure.
7. Use of Renewable Feedstocks
A raw material or feedstock should be renewable rather than depleting whenever technically and economically practicable.
8. Reduce Derivatives
Unnecessary derivatization (use of blocking groups, protection/deprotection, temporary modification of physical/chemical processes) should be minimized or avoided if possible, because such steps require additional reagents and can generate waste.
Catalytic reagents (as selective as possible) are superior to stoichiometric reagents. 10. Design for Degradation
Chemical products should be designed so that at the end of their function they break down into innocuous degradation products and do not persist in the environment.
11. Real-time analysis for Pollution Prevention
Analytical methodologies need to be further developed to allow for real-time, in-process monitoring and control prior to the formation of hazardous substances.
12. Inherently Safer Chemistry for Accident Prevention
Substances and the form of a substance used in a chemical process should be chosen to minimize the potential for chemical accidents, including releases, explosions, and fires.
As it can be observed, the 9th principle said that the utilization of catalysts is welcome, since typically catalysed reactions provides higher yield and selectivity. Often the best-performing catalysts are homogeneous, meaning that are in the same phase of the reactants. The classical example are soluble metal complexes, whose catalytic sites are all accessible and they grant the possibility to tune the chemo-, regio- and enantioselectivity of the catalyst.26 Moreover, homogeneous catalysts have a number of other advantages such as better yields, and easy optimization of catalytic systems by modification of ligand and metals. This catalyst category is extensively used in a number of commercial applications, but the problematic separation from the final product creates economic and environmental barriers to broadening their scope. Despite their advantages and their wide use, many homogeneous catalytic systems have not been commercialized because of the difficulty encountered in separating the catalyst from the final reaction product. Removal of trace amounts of catalyst from the target chemical is crucial since metal contamination is strongly regulated, especially in pharmaceutical industry. Even with the extensive and careful use of various techniques such as distillation, chromatography, or extraction, removal of trace amounts of catalyst remains a challenge. Evidently, the contamination issue is in contrast with the Green Chemistry policy and the necessity of further purification steps as well generates more wastes and increases the costs of the process. Moreover, homogenous catalyst are usually not reusable because of the recovery issues, which is cause of further increment of costs and resources utilization.
To overcome the separation problems in homogeneous catalysis, chemists and engineers have investigated a wide range of strategies and the use of heterogeneous catalyst systems looks as the best logical solution.27– 29 The common structural feature of these materials is the anchoring of the catalytic moiety on a scaffold that must have a good stability (thermal and chemical) and high surface area to ensure enough contact between active species and reactants (e.g. mesoporous silica scaffold).30,31 Anchoring can be achieved by covalent binding of the molecules or by simple adsorption, but covalent anchoring is clearly more robust and it can withstand harsh reaction conditions and it allows reusing the material several times. Although attempts have been made to make all active sites on solid supports accessible for reaction, allowing rates and selectivities comparable to those obtained with homogeneous catalysts, only sites on the surface are available for catalysis, which decreases the overall reactivity of the catalyst system. Therefore, the use of scaffolds that grant the best accessibility to catalytic centres is a smart route to push the application of heterogeneous catalysts.
In this view, 2D-Materials are very appealing just because of their bidimensional nature, which makes coinciding their surface chemistry with the bulk one and consequently making all the catalytic centres equally available. For instance, graphene combines this advantage to the typical characteristics required for a catalyst support such mechanical strength, tunable porosity and chemical inertness in most reaction media.32 Moreover, as will be discussed in section 1.3, graphene exhibits properties like high electronic33 and thermal conductivity,34–38 that can boost catalytic processes. A large variety of graphene derivatives has been developed recently, offering a large gamut of materials characterized by an extremely rich surface chemistry, which can be exploited for advanced functionalization protocols. Among these, graphene oxide (GO) is the most widely used, given its easy and scalable synthesis and because of plenty of surface oxygenated groups (i.e. tertiary alcohols, epoxide, carboxyl and carbonyl groups), 39 but other scaffold have been developed as well.
1.3 Evolution of 2D Materials and State of the Art1.3.1 First Generation of Graphene: Aiming the Perfection
The conceptual evolution on graphene was so intense and rich of extraordinary ideas that there have been three generations of graphene related materials with different properties, aims and purposes in less than 15 years. Indeed graphene started to be discussed theoretically since the 1947 by Wallace,40 but it took almost 60 years to isolate the first sample to characterize experimentally. At the discovery of Flatland, the outstanding properties of graphene came out instantly: for instance, high optical transparency (ca. 98% of transmitted light in the visible range),41,42 superior and anisotropic thermal conductivity (up to 2500 W·m-1
·K-1)34–38 and the highest mechanical strength ever measured (1 TPa Young’s modulus and 130.5 GPa tensile strength)43 made immediately appear graphene as a revolutionary material. Nevertheless, the more intriguing properties were uncovered when the electronic structure was studied. According to its band structure, graphene was found to be a zero-gap semiconductor, since valence and conduction bands meet at the six K-points of the Brillouin zone, generating the so-called Dirac cones structure.6,33,44–47 Thanks to the linear dispersion relation, graphene exhibits a huge in-plane carrier mobility, because fermions results to be substantially massless, allowing the hole and electron mobility to exceed 15000 cm2
·V-1·s-1.33 The combination of these properties made the material appearing as ideal for application in microelectronics, such as fabrication of ultrathin field effect transistors, inducing physics community to take the lead of graphene research main lines. Indeed, after finding that the dominant scattering mechanism is the one from defects and that the intrinsic limits of room temperature mobility is 2·105 cm2⋅V−1⋅s−1, the research focused on scaling up the production and on obtaining the most perfect graphene possible, with the aim of getting as near as possible to the hypothetical limit.48
1.3.2 Second Generation of Graphene: Chemically Modified and 3D-Structured Graphene
From the chemical point of view, defects are high-energy spots in the material scaffold that may be exploited to catalyse chemical or electrochemical reactions. Moreover, the theoretical surface area of monolayer graphene was calculated to be 2630 m2/g, a huge value that, combined with graphene electronic properties, makes this material an ideal support for catalysts and other materials to use in energy conversion and storage.49 Therefore, Material Scientists began a parallel study (that is Second Generation Graphene) on methods to prepare graphene in suitable quantities to use in the typical wet chemistry procedures. The following natural step was to insert intentionally defects in controlled ways in order to tune graphene properties with the aim, in this case, to enhance the catalytic properties.50 These studies allowed to develop a wide gamut of techniques to obtain larger and more processable quantities of modified graphene, with tunable properties and higher defectivity. Roughly, materials that came out from these second research branch may be divided in two main categories:
► Chemical Modified Graphene (CMG), that are materials made of graphene sheets modified by doping, so with relatively small quantity of substitutional heteroatoms (B, N, S, P,…) or even decorated with different functional groups;51–53
► 3D Graphene Architectures (3DG), where graphene or CMG morphology is controlled in order to obtain a three-dimensional network, for instance to expose higher active area, to activate some
catalytic sites or in general to use as base for more complex hybrids.54
Surely the most popular CMG is Graphene Oxide (GO): being typically produced by modified Hummer’s method,55 that consists of treating graphite with strongly oxidizing agents (such as H
2SO4, H3PO4, H2O2 and KMnO4), GO usually shows different functional groups on its surface, like epoxides, hydroxyl, carbonyl and carboxylic acid moieties.56 The presence of these oxygenated groups makes graphene sheets much more processable, since the increased polarity allows to suspend GO in polar solvent such as water, N,N-dimethylformamide (DMF) and N-methylpyrrolidone (NMP). The defectivity of GO tends to hamper the properties promoted by crystallinity (i.e. electrical conductivity), but they can be restored by reducing GO to reduced-GO (rGO) following several different methods (chemical, electrochemical or thermal). For this flexibility, GO actually became the benchmark for graphene-like materials. The main disadvantage of GO is however is ill-defined structure and inhomogeneity.
Very recently, another surface functionalized CMG, conceptually similar to GO, has been prepared, the so-called Graphene Acid (GA), synthesized by Otyepka and coworkers.57 GA is prepared from commercial fluorographite, whose C-F bonds undergo to nucleophilic substitution by reacting with sodium cyanide, giving the intermediate cyanographene. In the following step, nitrile moieties are converted to –COOH via acidic hydrolysis. Thanks to this well-designed synthesis route, GA has more homogeneous surface functionalization compared to GO, both as composition (mainly –COOH are present) and as distribution, being distributed uniformly on basal plane, in contrast with GO where functional moieties are especially on the edges. More interestingly, GA combines high surface functionalization with excellent electrical properties, comparable to rGO. Hence, GA is, in principle, a perfect substrate for catalyst heterogenization, giving an elegant example of how conventional chemistry can be applied on graphene to obtain the aimed properties.
The other family in CMGs is heteroatoms-doped graphene, where, instead of acting on surface functionalization, atoms like B, N, S, P are inserted in substitutional position in the graphene sheet.52,53,58–61 As for other semiconductor, the introduction of the heteroatom may strongly influence the electronic properties, for instance giving a preferential conductivity (n or p-type) and generating defects that can catalyse chemical or electrochemical reactions.
Among doped graphene materials, certainly N-doped graphene is the more deeply investigated.62–64 Typically, N-Graphene has been produced by Chemical Vapour Deposition (CVD) methods (annealing of GO or graphene in NH3 or other precursors), in solution or via electrochemical reduction.
Figure 1.3. Schematic representation of N-doped graphene with highlighted the typical defects produced in
the honeycomb lattice. Reproduced from ref. 21.
As shown in Figure 1.3, several kind of defects can be generated in the lattice and actually one of the challenges of this materials is to generate selectively just one type of defect, even if some procedure to obtain prevalent pyridinic or quaternary N-doping have been developed in recent years.65,66 This achievement is very important, since it has been proven that these defects can be exploited in appropriate applications, since, for instance, graphitic nitrogen is the main responsible for the n-conductivity of N-graphene and pyridinic nitrogen was found to be an active site for Oxygen Reduction Reaction (ORR).66
As mentioned above, the other massive category of materials of Second Generation Graphene is the 3D-Graphene Architectures (3DG). In the case of 3DG, graphene or CMG are shaped in order to exploit the properties of graphene in systems with high surface area. The prototypical 3DG is graphene aerogel produced by freeze-drying or supercritical CO2 drying of CMG suspension, generating self-standing 3D-networks with Brauner-Emmett-Teller (BET) surface area higher than 1000 m2/g.67–71 However, even other structures can be synthesized, like hollow nanospheres, crumpled sheets and capsules.54,72–76
Often, metallic templates have been used to shape up 3DGs: for instance, commercial Ni foams were used to produce supported graphene networks that, thanks to ultra-low density and high electrical conductivity, are appealing composites for a wide range of applications, like electrodes, supercapacitors and batteries.77– 79
In other cases, metals are used as sacrificial templates, so are chemically removed after synthesis in order to further increase the exposed area of the graphene. Nice examples are the works from research groups of Choi and Qu.80,81 In the early case, Ni nanoparticles (NPs) were coated with a polyol molecules, that were incorporated in the NiNPs by carburization at 250 °C. The following steps, annealing at 500 °C and treatment in HCl, allowed to form the multi-layer graphene on NiNPs surface and dissolve the template, respectively, achieving the final hollow graphene spheres. In the work of Qu, GO suspension was put in a glass pipeline, where a Cu wire was previously inserted. To form the extremely sharp shaped microtubes presented, the
glass pipeline was heated at 230 °C to hydrothermally reduce GO, followed by a treatment in aqueous FeCl3 to dissolve the Cu. This strategy allowed the authors to grow metal NPs selectively on the outer or on the inner wall, paving the way to multiple functionalities integrated on the same 3DG.
Clearly, these strategies are just some examples of an impressive number of papers in literature for preparing 3DGs and, in principle, each of these strategies can be applied to all CMGs with a huge number of possible combinations, depending on the final application the material is aimed to.
It is quite evident that CMGs and 3DGs are more relevant for energy applications compared to First Generation Graphene. The fine tuning of morphological, structural and electronic properties grants the possibility to adapt these materials to different research scopes, like the already mentioned catalysis, electrocatalysis, supercapacitance and other forms of energy storage and conversion. Naturally, the extreme flexibility exhibited by graphene-based materials put in the spotlight also other 2D layered materials and transferring the knowledge acquired from graphene to other 2D-materials pulled the trigger on the Third Generation Graphene.
1.3.3 Third Generation of Graphene: Graphene Related Materials
Despite the outstanding properties shown by graphene, CMGs and 3DGs, it was unavoidable to face a failure in some applications. Curiously, graphene is still missing promises in one of the earlier application of the First Generation, which is the use as channel material in Field Effect Transistors (FETs). Indeed, the electronic properties that attracted electron-device community are also the main issue for FET applications. Briefly, as showed by Schwierz,82 if graphene is used as channel semiconductor, it becomes troublesome to turn off the FET, since the absence of the band gap implies that, even if no potential is applied to the FET gate, the material switches from electron to hole conductivity instead of stopping the carriers flow. The consequence is the On/Off current ratio was found to be between 2 and 20, which is completely insufficient considering that the minimum recommended value is 103. In principle, using CMGs is possible to tune the gap from 0 to 0.5 eV, but On/Off current ratio is still far from values suitable for practical applications and for competing with mainstream silicon technologies.83 The immediate consequence was that other “continents” of the
Flatland started being explored in order to have a channel material with a real band gap, but also some
fascinating properties of 2D-materials like the definite layer structure without dangling bonds and atomic-level thickness.
Even if this is just an example, a similar evolution occurred also in other research fields. In electrocatalysis, graphene itself showed bad activity in electrochemical WS, having actually no active sites for Hydrogen Evolution Reaction (HER) and Oxygen Evolution Reaction (OER). Ab initio calculations84 showed that better performances could be obtained by coupling graphene with metal surfaces or by using CMGs, since the interruption of the lattice due to the presence of heteroatoms may acts as catalytic site for WS. However, it has to be considered that not all the defects are prone to perform the same electrocatalytic reaction, so chemical modification has to come together with a fine defects tuning in order to obtain competitive performances. For these objective difficulties, very few works have been published on the experimental utilization of pure CMGs in electrochemical WS. Zhang and Dai recently prepared and tested N,P,F-Tri-doped graphene as multifunctional catalyst for ORR and WS,85 but more than 2 V were necessary to drive 10
mA/cm2, that is 0.8 V above the thermodynamical limit of 1.23 V for WS. Better results were obtained in Yao’s research group, where graphene with high concentration of topological defects was synthesized and tested for ORR and overall WS.86 With respect to previous case, defective graphene in WS needs 0.6 V overpotential to reach 10 mA/cm2, that it is a good result for a metal-free catalyst, but far from the benchmarks, especially in alkaline HER. Consequently, at the state of the art of WS, graphene and CMGs are mostly used as support for other metal-based materials, with the aim of exploiting electrical properties or to implement some synergies by forming a junction with the active material.
As demonstrated by these cases, graphene and CMGs, even if revolutionary materials, are not the magic bullet to all the challenges that scientific community has been facing in the last decade. However, the impressive knowledge acquired on graphene was decisive in processing, characterizing and improving performance of the other 2D-materials. Actually, graphene-related materials (GRMs) are complementary to graphene: GRMs are associated to CMGs and graphene being layered, on the other hand they have completely different electronic structure and chemical composition. The most notorious members of GRMs family are depicted in Figure 1.4.
As written above, all these materials have some common peculiarities due to their 2D nature: ► Atomic-level thickness;
► Definite layer structure;
► No dangling bonds: carriers conducted on the surface of the material encounter very low roughness, reducing the scattering probability;
► Tunability of optoelectronic properties with of layers;
► Application of similar protocols for processing materials (e.g. exfoliation, purification, morphology modification).
However, their chemical composition is really very heterogeneous: Graphitic Carbon Nitride (g-C3N4) is still a carbon based materials, Hexagonal Boron Nitride (h-BN) and Phosphorene has no carbon in their structures but they are metal-free, Transition Metal Dichalcogenides (TMDCs) and layered MnO2 can exploit the chemistry of metals, but being chalcogenides and oxides, respectively, direct them in completely different applications. Curiously, considering graphene, CMGs and GRMs, 2D semiconductors band gaps can cover continuously the energy range from 0 to 2.6 eV (from far-IR to cyan light) plus an insulator like h-BN (ca. 5.9 eV),87 giving a wide selection of optoelectronic properties for the use of 2D-materials in specific applications (see Figure 1.5).
Figure 1.5. Schematic diagram of 2D-Materials band gaps. Reproduced from 57.
Among GRMs, Graphitic Carbon Nitride (g-C3N4) can be considered the most similar to graphene, since its structure can be associated with that of a strongly N-doped graphene. g-C3N4 is a good electrocatalyst and, thanks to its 2.6 eV band gap, its performances can be boosted via visible light irradiation.88,89 For instance, g-C3N4 is a promising catalysts for the ORR due to the high content of pyridinic and graphitic N and abundant edge amine sites, but it was also successfully tested in photocatalytic CO2 Reduction Reaction (CRR) to further processable organic feedstocks (CO, formic acid, formaldehyde,…).90,91 Moreover, the natural vacancies in g-C3N4 can be patched by growing highly monodispersed nanoparticles, resulting in interesting synergistic effects.88 However, g-C
3N4, being a sort of defective graphene, suffers of poor electronic conductivity, limiting large scale applications, so this material is often used in combination with conductive 2D-materials (i.e. graphene or CMGs) in order to improve electrochemical performances.92
Also h-BN has the same honeycomb lattice of graphene and it is isoelectronic as well, but the polar nature of B–N bonds make the band gap to pass from 0 to almost 6 eV. Obviously, the insulating behaviour of h-BN seriously hamper applications in electrochemistry, so it is mostly used as dielectric substrate for other GRMs or as substitute of SiO2 in all-2D FETs.93–95 However, recent works showed that via chemical doping is possible to reduce the h-BN gap down to 2 eV.96
Phosphorene is the black allotrope of phosphorous, reduced to the monolayer thickness. Phosphorene structure notably differs from graphene’s honeycomb, because of the presence of 5 electrons in P 3p orbitals that gives rise to sp3 hybridization, explaining the non-planarity of the 2D sheet.97 This particular GRMs is interesting because of the combination of a small band gap (from 0.3 eV in bulk to 1.88 eV in monolayer) with a good electrical conductivity.98 Indeed, in recent years some works have been published on the use phosphorene both as electrocatalyst and photoelectrocatalyst, showing some interesting results in HER and OER.99–101 Unfortunately, the main drawback of using black phosphorous in electrocatalysis is the low stability in atmospheric conditions, since it degrades in contact with water and oxygen, which is also a visible light pronounced process. Therefore, at the moment, the main application scopes of phosphorene are the ones in controlled atmosphere, like fabrication of FETs and batteries.102,103
δ-MnO2 is the only layered of six polymorphs of MnO2, and it comes with a 2.1 eV band gap in bulk crystals,104,105 meaning that this oxide may be used as visible light activated photocatalyst.106 Interestingly, δ-MnO2 tends to intercalate cations and water molecules in the interlayer space, modifying both the band gap and the electrochemical performances.106 Being an oxide, δ-MnO
2 suffers of low conductivity, but compared with other GRMs it exhibits excellent stability in oxidative conditions.107 Therefore, δ-MnO
2 has been found to catalyse OER and photo-OER with moderate overpotentials.105,108,109 However, δ-MnO
2 catalytic activity is not limited to water oxidation, but it was found to be a well-performing catalyst also in ORR and in other reactions, like formaldehyde oxidation.107,110 Typically, δ-MnO
2 was considered to be inactive for the WS cathodic half-reaction, due to its unsuitable electronic structure and low conduction band level. However, as demonstrated by the Second Generation of Graphene, defects engineering can pave the way to generate new active sites in the same material, and this was for MnO2. Wang et al. observed half-metallic character in monolayer nanosheets doped with Mn and O vacancies, a property not observed in bulk counterparts, providing a new strategy for improving the electronic properties and conductivity of δ-MnO2 for overall WS.111 In a following work, Zhao et al. synthesized a hierarchical composite δ-MnO
2/Ni-foam with high vacancies abundance:112 during tests for WS, a remarkable 0.5 V global overpotential at 10 mA/cm2 was recorded, with about 560 mV improving of HER onset with respect to bulk δ-MnO2.
Finally, TMDCs are the most investigated GRMs (together with graphene-based materials), as established by the about 104 publications in 2016.102 TMDCs are a wide family of materials with a common rough formula MX2 (M = Mo, W, V, Nb, Ta, Ti, Re, Zr,… and X = S, Se or Te) and a sandwich-like hexagonal structure with a layer of metal atoms enclosed between two chalcogenide atoms layer (see Figure 1.4). Consequently, with respect to most GRMs, in TMDCs there is possibility to tune optoelectronic properties also by composition: considering the prototypical TMDC (i.e. MoS2), studies were carried out to proof the excellent controlling of properties by making alloys mixing both metals (e.g. Mo(1-x)WxS2) and chalcogenides (e.g. MoS2(1-x)Se2x),113–118 coming up with precise band gap engineering and modulation of related properties, like photoluminescence.
Moreover, all TMDCs has more than one polymorph, with different properties and activities, and also amorphous material were found to be very active in some electrocatalytic reactions. Considering again MoS2, it can exist in three polymorphic forms, schematically represented in Figure 1.6. The most common is the hexagonal 2H-phase, which exhibits semiconducting behaviour with band gap from 1.2 to 1.9 eV when decreasing the number of layers. The distorted tetragonal 1T-phase is typically obtained upon alkali intercalation and following exfoliation into nanosheets, it is metallic and basically metastable and very defective, characteristics that grant to this polymorph to perform extremely well in HER.20,119 The rarest polytype is the rombohedral 3R-phase, that has to be synthesized through specific growing procedures and behave like a semiconductor (indirect band gap 1.3 eV).120–122 Each of these polymorphs possesses unique structures and electronic properties from where different catalytic properties can emerge due to the different active sites.
Figure 1.6. 3D models of different 1T, 2H and 3R MoS2 polymorphs, respectively. The symmetry group of the crystallographic unit cell is reported in brackets.
Moreover, amorphous MoS2 and non-stoichiometric MoSx (2 < x < 3) can be easily synthesized from suitable precursors and, thanks to high number of defects, they may have different active sites, exhibiting also in this case very interesting activity in electrocatalysis.123–126
It is quite evident that the intrinsic activity of TMDCs, combined with the huge tuning possibilities, is the reason for the high focus on these GRMs, considering that all the strategies applicable to other 2D-materials can be actualized (i.e. doping, 3D-structuring, hybrids, …) as well. Actually, the application of TMDCs spans substantially in every field where an electroactive material is required, thanks to their versatility comparable to graphene one. For example, in microelectronics field MoS2 has been successfully tested as channel material in FETs and logic devices,94,95,127–129 and as part of MoS
memory cells130 and photodetectors.131 Similarly, TMDCs were largely tested in lithium ion batteries132–134 and supercapacitors,20,135–138 taking advantage of all the approaches developed for graphene and CMGs for selectively improving the required properties. Concerning electrocatalysis, TMDCs are among the benchmark materials in HER. Indeed, especially MoS2 and MoSe2 based electrocatalysts exhibited extremely good performances even if the HER reaction was mostly tested in not ideal conditions (i.e. in basic electrolyte). Considering HER in the typical conditions (0.5 M H2SO4), it is well-known that 1T-MoS2 can perform HER with low overpotentials and kinetics close to Pt, which is believed being related to the high number of defects generated during the stressing exfoliation process.119 Another example is a 3D-structured composite prepared by growing MoS2(1-x)Se2x on a selenized Ni-foam. Even if three steps were necessary to achieve the final material, an outstanding 69 mV overpotential was sufficient to draw 10 mA/cm2 and about 110 mV for 100 mA/cm2.139 In OER the activity of MoS
2 is low due to a certain lack of stability, but a nice work from Mattevi’s group showed improved performance making a bulk heterojunctions combining MoS2 and WS2.140 Finally, TMDCs showed excellent performances also in CRR, with just the help of some ionic liquid in the electrolyte to suppress HER, being two competitive process in the same potential window.141,142 In this case the best performing material was found to be WSe2, whose overpotential for CRR was found to be 54 mV.
1.4 Ph.D. Thesis Structure
This Ph.D. project, as extensively discussed in section 1.2, is aimed to discover new strategies to develop materials to utilize in the fields of Green Energy and Green Chemistry and it was directed at the application of 2D Materials in particular. Section 1.3 reported part of the huge work made by scientific community on these materials and underlined the still unexpressed potential that lies in them.
In our studies in the Green Energy area, we focused on the use of MoS2-based materials in WS cathodic half-reaction in order to obtain the best possible performance in hydrogen generation in different conditions. To do that, different strategies were developed (i.e. metal doping, inorganic and organic/inorganic hybrids) to drive the original material to adapt to specific application.
Regarding Green Chemistry area, we used a specific CMG, that is the already mentioned Graphene Acid (GA), and we exploited its uniform surface functionalization to prepare materials for heterogeneous catalysis for different reactions, comparing them with the benchmark GO, modified with the same protocol.
The Thesis work is divided in 5 main chapters. In Chapter Two we investigated the design of three-dimensional MoS2 structures doped with several amount of Ni in order to activate MoS2 for the HER performed in alkaline environment, which typically hinder this reaction. Nevertheless, the introduction of a different cation in the lattice can causes the modification of the structure, which can also influence the HER. We prepared 3D-structured MoS2 samples (hereafter 3D-MoS2) obtained starting from ammonium tetrathiomolybdate (ATM) using a procedure that also allows to easily introduce the dopant in a single pot. We tested several conditions in order to find the procedure that would allow to expose as much active sites as possible. We then studied the effects of different amount of Ni doping both on the 3D-MoS2 structure and the catalytic performances in HER, both in acidic and in basic media. The investigation was carried on combining several techniques. Morphology was examined by electronic microscopies, both Scanning (SEM) and Transmission Electron Microscopy (TEM). During the same measurements, we also performed Energy
Dispersive X-Ray analysis (EDX) to verify the effective distribution of the dopant, since eventual inhomogeneity would indicate the segregation of distinct dopant-based species (MxOy or MxSy), a process that may happen especially with relatively high loadings. The influence of Ni on MoS2 lattice was investigated by mean of X-Ray Diffraction Analysis (XRD) and Raman Spectroscopy. The combination of these techniques was helpful to reveal the dopant influence on the lattice parameters and the defectivity and stacking of the MoS2 layers. X-Ray Photoemission Spectroscopy (XPS) was decisive in bridging the structural information with HER activity. Indeed, XPS was helpful to observe the dopant chemical environment, figuring out the different kind of active sites produced on the material. Moreover, the shifts in Binding Energy (BE) of the signals relative to the scaffold showed how the dopant influenced the MoS2 electronic structure. We performed an extensive electrochemical characterization in acidic (0.5M H2SO4) and alkaline (1.0M KOH) electrolytes to find out the role of each active species in catalysing HER depending on the available species to react, both in terms of pure performances and of reaction kinetics. The result was a contrasting behaviour of the materials due to the different abundance of active sites generated by Ni on MoS2 edge or basal plane.
In Chapter Three, we developed a method for preparing amorphous MoS2/Ag2S hybrid using recycled DVD as the substrate; this revealed as a viable opportunity to turn an abundant waste into an added-value material. We produced the hybrid materials by exposing the Ag patterned layer of commercial DVD and by electro-depositing the material from a 50 mM ATM aqueous solution for 3 minutes. The reduction of ATM simultaneously cause the deposition of MoS2 and the generation of SH- anions that sulphidize metallic Ag to Ag2S, forming MoS2/Ag2S n-p nanojunctions. To proof the role of MoS2, we grown pure Ag2S and MoO2 films as blank experiments. The evolution of the DVD support was followed by using SEM, XRD and Raman Spectroscopy, for morphology, crystal phases and structural modifications, respectively. SEM showed a strongly increased roughness of the DVD substrate, while XRD and Raman measurements revealed the amorphous nature of materials deposited through this protocol. XPS further confirmed the amorphous nature of the films and allowed to quantify the ratio among the sulphides. We operated electrochemical tests by combining polarization curves, Electrochemical Impedance Spectroscopy (EIS) and double-layer capacitance measurements, resulting in a very cheap and effective catalyst for HER. Moreover, thanks to the presence of n-p junctions (proofed by Mott-Schottky analysis), a nice 10% performance enhancement under visible light irradiation was observed.
In Chapter Four another kind of hybrid was prepared by designing a one-pot hydrothermal synthesis of MoS2(1-x)Se2x nanosheets grown on N-doped reduced Graphene Oxide (hereafter N-rGO). This study was focused on optimizing a synthesis that allows a precise and easy-to-tune Se:S ratio, with the goal of controlling optoelectronic properties. In the synthesis we utilized ATM as MoS2 precursor in the presence of Dimethyl Diselenide (DMDSe) as selenizing agent. Through a series of blank experiments, we found that a two-temperatures synthesis was the best to obtain the target material: a first step at 180°C to allow the growth of MoSx slabs without the competition with selenization reaction and subsequently a step at 200 °C to activate DMDSe and substituting S anions on the nanosheets. The materials that we obtained were found to be amorphous due to low process temperature. Therefore two different goals were chased: the as-produced materials were tested for HER in acidic environment, while crystalline materials, obtained by annealing at 600 °C, were destined to photoinduced HER. The reason resides on the different crystallinity: the amorphous samples, being highly defective, were expected to have higher intrinsic catalytic activity but
worse interaction with light because of defects-mediated exciton recombination; on the other hand, crystallizing the materials would allow losing pure performance but improving the exciton lifetime, favouring the photoinduced reaction. Indeed, this hybrid material is based on the interaction between two moieties that are responsible for the creation of a p-n nanojunction and have two synergistic roles (imparting good electric conduction the N-rGO, and granting a low overpotential the MoS2(1-x)Se2x) inside a unique catalytic reaction. The tuning of Se:S ratio was followed by the evolution of Raman modes with the changes in composition, as in the case of XPS, that was used to determine the Se:S ratio. HER activity and kinetics was firstly investigated for all the produced samples, revealing that, in the case of amorphous samples, the introduction of Se had no beneficial effects, since amorphous MoS2/N-rGO was the best performing material. On the other hand, after annealing the intrinsic defectivity of Se-containing samples completely reverted the trends. Subsequently, photoinduced HER was studied for selected samples: as expected, amorphous samples were found to be much less responding to light irradiation compared to crystalline counterparts. On the latter, UV-Vis, transient photocurrent and Incident Photons to Current Efficiency (IPCE) studies were made to observe the evolution of performance with different Se contents.
The contents of Chapter Five move from electrocatalysis to heterogeneous catalysis. We synthesized a heterogeneous catalyst by covalently grafting Ferrocene (Fc) moieties to –COOH surface groups of GA and GO. The resulting Fc-modified graphene derivatives have been tested as heterogeneous catalysts for the C-H insertion of aryl diazonium salts into several arene substrates, a reaction of pivotal importance for organic chemistry since it activates a rather inert system, opening new reaction pathways in the synthetic research. The materials were extensively characterized along every synthetic step. SEM and TEM experiments were performed to check the morphology, Raman spectroscopy was used to calculate the ID/IG ratio and we observed in UV-Vis spectra the appearance of Fc bands. Thanks to XPS measurements we were able to follow the evolution of C core level along the functionalization steps. XPS was used as well to determine the amount of Fe in the final materials, crosschecking the results with EDX analysis and with charge integration measurement in Cyclic Voltammetry (CV) experiments. Once the successful functionalization of the GA and GO supports with Fc was demonstrated, and considering that molecular Fc shows a good catalytic activity in the C-H insertion of diazonium salts into arene substrates reaction, the GA- and GO-based materials were tested as heterogeneous catalysts for the same reaction. The catalytic activity and kinetics were observed via Nuclear Magnetic Resonance (NMR), resulting not only in a successful heterogenization of Fc, but also in a clear superiority of GA as scaffold with respect to GO.
A different type of graphene-based catalyst was investigated in Chapter Six, in particular we have grown Pd nanoparticles on GA and GO to create a material for Suzuki-Miyaura cross coupling reaction. The literature is full of reports where researchers tackle the combination of Pd and graphene in form of small metallic dots, with diameter ranging from big clusters (less than 2 nm) to big nanoparticles (80-100 nm). However, the mechanism on how the nanoparticles grow on surface is not addressed. It is believed that surface oxygen groups on GO or rGO play a role. In order to shed light about this fundamental question, we employed GA as platform to grow Pd nanoparticles. The uniform surface chemistry become crucial to understand the chemical transformation involved in the nucleation and growing of the supported metallic nanoparticles. We characterized the synthesized materials by mean of XPS, which was essential in observing the changings of C line upon impregnation and of Pd core level, where both chemical state and capacitive effects due to
quantum confinement could be observed. Moreover, an estimation of Pd loading could be calculated and further confirmed by EDX and Inductively Coupled Plasma Mass Spectrometry (ICP-MS). On GA, different Pd loadings were essayed to obtain smaller (i.e. more active) Pd nanoparticles. TEM analysis demonstrated that much narrower Pd nanoparticles size distribution could be obtained on GA with respect to GO, proofing the importance of surface moieties in controlling nanoparticles growth. Also UV-Vis spectroscopy confirmed these hypothesis, since it is known that the size of the Pd nanoparticle can affect the optical properties regarding the corresponding maximum of the plasmonic effect. Regarding the catalytic activity, the Suzuki-Miyaura reaction is one of the most widespread employed cross-coupling reactions to form C-C bonds. Pd nanoparticles supported on graphene derivatives have already been reported to have activity on the cross coupling of boronic acids with different halides, demonstrating good catalytic performance with high stability, cyclability and versatility even working under green conditions. Other authors, however, reported the synthesis of homocoupling catalysts of boronic acids instead of the cross-coupling ones. Thanks to Pd nanoparticles homogeneity, derived from uniform surface functionalization of GA, we found that our GA-Pd system is able to perform selectively and in green conditions both reactions with a simple control of the reagents involved.
(1) International Energy Agency. World Energy Outlook (WEO) www.iea.org/weo.
(2) United Nations Environment Programme. Division of Technology, I. Hydrogen Economy : A
Non-Technical Review.; 2006.
(3) McDowall, W.; Eames, M. Forecasts, Scenarios, Visions, Backcasts and Roadmaps to the Hydrogen Economy: A Review of the Hydrogen Futures Literature. Energy Policy 2006, 34 (11), 1236–1250. (4) Balasubramanian, B.; Ortiz, A. L.; Kayatakoglu, S.; Harris, D. P. Hydrogen from Methane in a
Single-Step. Process. Chem. Eng. Sci. 1999, 54, 3543.
(5) Faber, M. S.; Jin, S. Earth-Abundant Inorganic Electrocatalysts and Their Nanostructures for Energy Conversion Applications. Energy Environ. Sci. 2014, 7 (11), 3519–3542.
(6) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; D. Jiang, Y. Z.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. Electric Field Effect in Atomically Thin Carbon Films. Science 2004, 306 (5696), 666–669.
(7) Zurutuza, A.; Marinelli, C. Challenges and Opportunities in Graphene Commercialization. Nat.
Nanotechnol. 2014, 9 (10), 730–734.
(8) Ren, W.; Cheng, H. M. The Global Growth of Graphene. Nat. Nanotechnol. 2014, 9 (10), 726–730. (9) Ellabban, O.; Abu-Rub, H.; Blaabjerg, F. Renewable Energy Resources: Current Status, Future Prospects
and Their Enabling Technology. Renew. Sustain. Energy Rev. 2014, 39, 748–764.
(10) Xia, W.; Mahmood, A.; Liang, Z.; Zou, R.; Guo, S. Earth-Abundant Nanomaterials for Oxygen Reduction.
Angew. Chemie - Int. Ed. 2016, 55 (8), 2650–2676.
(11) Shao, M.; Chang, Q.; Dodelet, J.-P.; Chenitz, R. Recent Advances in Electrocatalysts for Oxygen Reduction Reaction. Chem. Rev. 2016, 116 (6), 3594–3657.
(12) Xia, B. Y.; Yan, Y.; Wang, X.; Lou, X. W. Recent Progress on Graphene-Based Hybrid Electrocatalysts.
Mater. Horizons 2014, 1 (4), 379–399.
(13) European Commission. Critical Raw Materials ec.europa.eu/growth/sectors/raw-materials/specific-interest/critical_en.
(14) Mathieux, F.; Ardente, F.; Bobba, S.; Nuss, P.; Blengini, G.; Alves Dias, P.; Blagoeva, D.; Torres De Matos, C.; Wittmer, D.; Pavel, C.; Hamor, T.; Saveyn, H.; Gawlik, B.; Orveillon, G.; Huygens, D.; Garbarino, E.; Tzimas, E.; Bouraoui, F.; Solar, S. Critical Raw Materials and the Circular Economy -
Background Report; 2017.
(15) Muradov, N. Z.; Veziroǧlu, T. N. From Hydrocarbon to Hydrogen-Carbon to Hydrogen Economy. Int. J.
Hydrogen Energy 2005, 30 (3), 225–237.
(16) Cheng, Y.; Jiang, S. P. Advances in Electrocatalysts for Oxygen Evolution Reaction of Water Electrolysis-from Metal Oxides to Carbon Nanotubes. Prog. Nat. Sci. Mater. Int. 2015, 25 (6), 545–553.
(17) Meyer, T. J. The Art of Splitting Water. Nature 2008, 451, 778.
(18) Tao, H.; Gao, Y.; Talreja, N.; Guo, F.; Texter, J.; Yan, C.; Sun, Z. Two-Dimensional Nanosheets for Electrocatalysis in Energy Generation and Conversion. J. Mater. Chem. A 2017, 5 (16), 7257–7284. (19) Tan, C.; Cao, X.; Wu, X.-J.; He, Q.; Yang, J.; Zhang, X.; Chen, J.; Zhao, W.; Han, S.; Nam, G.-H.; Sindoro,
M.; Zhang, H. Recent Advances in Ultrathin Two-Dimensional Nanomaterials. Chem. Rev. 2017, 117 (9), 6225–6331.